• ### Energy Gap Evolution Across the Superconductivity Dome in Single Crystals of (Ba$_{1-x}$K$_x$)Fe$_2$As$_2$(1605.04183)

Oct. 12, 2016 cond-mat.supr-con
The mechanism of unconventional superconductivity in iron-based superconductors (IBSs) is one of the most intriguing questions in current materials research. Among non-oxide IBSs, (Ba$_{1-x}$K$_x$)Fe$_2$As$_2$ has been intensively studied because of its high superconducting transition temperature and fascinating evolution of the superconducting gap structure from being fully isotropic at optimal doping ($x\approx$0.4) to becoming nodal at $x >$0.8. Although this marked evolution was identified in several independent experiments, there are no details of the gap evolution to date because of the lack of high-quality single crystals covering the entire K-doping range of the superconducting dome. We conducted a systematic study of the London penetration depth, $\lambda (T)$, across the full phase diagram for different concentrations of point-like defects introduced by 2.5 MeV electron irradiation. Fitting the low-temperature variation with the power law, $\Delta \lambda \sim T^{n}$, we find that the exponent $n$ is the highest and $T_c$ suppression rate with disorder is the smallest at optimal doping, and they evolve with doping being away from optimal, which is consistent with increasing gap anisotropy, including an abrupt change around $x\simeq 0.8$, indicating the onset of nodal behavior. Our analysis using a self-consistent $t$-matrix approach suggests the ubiquitous and robust nature of s$_{\pm}$ pairing in IBSs and argues against a previously suggested transition to a $d-$wave state near $x=1$ in this system.
• ### Variation of transition temperatures and residual resistivity ratio in vapor-grown FeSe(1606.00500)

June 1, 2016 cond-mat.supr-con
The study of the iron-based superconductor FeSe has blossomed with the availability of high quality single crystals, obtained through flux/vapor-transport growth techniques below the structural transformation temperature of its tetragonal phase, T~450 C. Here, we report on the variation of sample morphology and properties due to small modifications in the growth conditions. A considerable variation of the superconducting transition temperature Tc, from 8.8 K to 3 K, which cannot be correlated with the sample composition, is observed. Instead, we point out a clear correlation between Tc and disorder, as measured by the residual resistivity ratio. Notably, the tetragonal-to-orthorhombic structural transition is also found to be quite strongly disorder dependent (Ts =72 - 90 K), and linearly correlated with Tc.
• ### Remarkably robust and correlated coherence and antiferromagnetism in (Ce$_{1-x}$La$_x$)Cu$_2$Ge$_2$(1412.2092)

Aug. 31, 2015 cond-mat.str-el
We present magnetic susceptibility, resistivity, specific heat, and thermoelectric power measurements on (Ce$_{1-x}$La$_x$)Cu$_2$Ge$_2$ single crystals (0 $\leq x\leq$ 1). With La substitution, the antiferromagnetic temperature $T_N$ is suppressed in an almost linear fashion and moves below 0.36 K, the base temperature of our measurements for $x>$ 0.8. Surprisingly, in addition to robust antiferromagnetism, the system also shows low temperature coherent scattering below $T_{coh}$ up to $\sim$ 0.9 of La, indicating a small percolation limit $\sim$ 9$\%$ of Ce that separates a coherent regime from a single-ion Kondo impurity regime. $T_{coh}$ as a function of magnetic field was found to have different behavior for $x$< 0.9 and $x$> 0.9. Remarkably, $(T_{coh})^2$ at $H$ = 0 was found to be linearly proportional to $T_N$. The jump in the magnetic specific heat $\delta C_{m}$ at $T_N$ as a function of $T_K/T_N$ for (Ce$_{1-x}$La$_x$)Cu$_2$Ge$_2$ follows the theoretical prediction based on the molecular field calculation for the $S$ = 1/2 resonant level model.
• ### Effects of electron irradiation on resistivity and London penetration depth of Ba$_{1-x}$K$_x$Fe$_2$As$_2$ ($x \leq$ 0.34) iron - pnictide superconductor(1408.0025)

July 31, 2014 cond-mat.supr-con
Irradiation with 2.5 MeV electrons at doses up to 5.2 $\times$10$^{19}$ electrons/cm$^2$ was used to introduce point-like defects in single crystals of Ba$_{1-x}$K$_x$Fe$_2$As$_2$ with $x=$ 0.19 ($T_c=$ 14 K), $x=$ 0.26 ($T_c=$ 32 K) and 0.34 ($T_c=$ 39 K) to study the superconducting gap structure by probing the effect of non-magnetic scattering on electrical resistivity, $\rho(T)$, and London penetration depth, $\lambda (T)$. For all compositions, the irradiation suppressed the superconducting transition temperature, $T_c$ and increased resistivity. The low - temperature behavior of $\lambda (T)$ is best described by the power - law function, $\Delta \lambda (T) = A(T/T_c)^n$. While substantial suppression of $T_c$ supports $s_{\pm}$ pairing mechanism, in samples close to the optimal doping, $x=$ 0.26 and 0.34, the exponent $n$ remained high ($n \geq 3$) indicating robust full superconducting gaps. For the $x=$ 0.19 composition, exhibiting coexistence of superconductivity and long - range magnetism, the suppression of $T_c$ was much more rapid and the exponent $n$ decreased toward dirty limit of $n$ = 2. In this sample, the irradiation also suppressed the temperature of structural/magnetic transition, $T_{sm}$, from 103 K to 98 K consistent with the itinerant nature of the magnetic order. Our results suggest that underdoped compositions, especially in the coexisting regime are most susceptible to non-magnetic scattering and imply that in multi-band Ba$_{1-x}$K$_x$Fe$_2$As$_2$ superconductors, the ratio of the inter-band to intra-band pairing strength, and associated gap anisotropy, increases upon the departure from the optimal doping.
• ### Resolution of the discrepancy between the variation of the physical properties of Ce1-xYbxCoIn5 single crystals and thin films with Yb composition(1407.6725)

July 24, 2014 cond-mat.str-el
Measurements of physical properties show that Yb enters the single crystals systematically and in registry with the nominal Yb concentration x of the starting material dissolved in the molten indium flux.
• ### Competition between superconductivity and magnetic/nematic order as a source of anisotropic superconducting gap in underdoped Ba$_{1-x}$K$_{x}$Fe$_{2}$As$_{2}$(1406.2369)

June 9, 2014 cond-mat.supr-con
The in-plane London penetration depth, $\Delta\lambda(T)$, was measured using a tunnel diode resonator technique in single crystals of Ba$_{1-x}$K$_{x}$Fe$_{2}$As$_{2}$ with doping levels $x$ ranging from heavily underdoped, $x$=0.16 ($T_{c}$=7~K) to nearly optimally doped, $x$= 0.34 ($T_{c}=$39 K). Exponential saturation of $\Delta\lambda(T)$ in the $T\to0$ limit is found in optimally doped samples, with the superfluid density $\rho_{s}(T)\equiv(\lambda(0)/\lambda(T))^{2}$ quantitatively described by a self-consistent $\gamma$-model with two nodeless isotropic superconducting gaps. As the doping level is decreased towards the extreme end of the superconducting dome at $x$=0.16, the low-temperature behavior of $\Delta\lambda(T)$ becomes non-exponential and best described by the power-law $\Delta\lambda(T)\propto T^{2}$, characteristic of strongly anisotropic gaps. The change between the two regimes happens within the range of coexisting magnetic/nematic order and superconductivity, $x<0.25$, and is accompanied by a rapid rise in the absolute value of $\Delta\lambda(T)$ with underdoping. This effect, characteristic of the competition between superconductivity and other ordered states, is very similar to but of significantly smaller magnitude than what is observed in the electron-doped Ba(Fe$_{1-x}$Co$_{x}$)$_{2}$As$_{2}$ compounds. Our study suggests that the competition between superconductivity and magnetic/nematic order in hole-doped compounds is weaker than in electron-doped compounds, and that the anisotropy of the superconducting state in the underdoped iron pnictides is a consequence of the anisotropic changes in the pairing interaction and in the gap function promoted by both magnetic and nematic long-range order.
• ### Interplane resistivity of underdoped single crystals (Ba$_{1-x}$K$_x$)Fe$_2$As$_2$, $0 \leq x<0.34$(1404.3664)

April 14, 2014 cond-mat.supr-con
Temperature-dependent inter-plane resistivity, $\rho _c(T)$, was measured in hole-doped iron-arsenide superconductor (Ba$_{1-x}$K$_x$)Fe$_2$As$_2$ over a doping range from parent compound to optimal doping $T_c\approx 38~K$, $0\leq x \leq 0.34$. Measurements were undertaken on high-quality single crystals grown from FeAs flux. The coupled magnetic/structural transition at $T_{SM}$ leads to clear accelerated decrease of $\rho_c(T)$ on cooling in samples with $T_c <$26~K ($x <0.25$). This decrease in hole-doped material is in notable contrast to an increase in $\rho_c(T)$ in the electron-doped Ba(Fe$_{1-x}$Co$_x$)Fe $_2$As$_2$ and iso-electron substituted BaFe$_2$(As$_{1-x}$P$_x$)$_2$. The $T_{SM}$ decreases very sharply with doping, dropping from $T_s$=71~K to zero on increase of $T_c$ from approximately 25 to 27~K. The $\rho_c(T)$ becomes $T$-linear close to optimal doping. The broad crossover maximum in $\rho_c(T)$, found in the parent BaFe$_2$As$_2$ at around $T_{max} \sim$200~K, shifts to higher temperature $\sim$250~K with doping $x$=0.34. The maximum shows clear correlation with the broad crossover feature found in the temperature-dependent in-plane resistivity $\rho_a(T)$. The doping evolution of $T_{max}$ in (Ba$_{1-x}$K$_x$)Fe$_2$As$_2$ is in notable contrast with both rapid suppression of $T_{max}$ found in Ba(Fe$_{1-x}TM_x$)$_2$As$_2$ ($TM$=Co,Rh,Ni,Pd) and its rapid increase BaFe$_2$(As$_{1-x}$P$_x$)$_2$. This observation suggest that pseudogap features are much stronger in hole-doped than in electron-doped iron-based superconductors, revealing significant electron-hole doping asymmetry similar to the cuprates. This paper replaces: cond-mat:1106.0533.
• ### A comprehensive scenario of the single crystal growth and doping dependence of resistivity and anisotropic upper critical fields in (Ba$_{1-x}$K$_x$)Fe$_2$As$_2$ ($0.22 \leq x \leq 1$)(1403.0227)

March 2, 2014 cond-mat.supr-con
Large high-quality single crystals of hole-doped iron-based superconductor (Ba$_{1-x}$K$_x$)Fe$_2$As$_2$ were grown over a broad composition range $0.22 \leq x \leq 1$ by inverted temperature gradient method. We found that high soaking temperature, fast cooling rate, and adjusted temperature window of the growth are necessary to obtain single crystals of heavily K doped crystals (0.65$\leq x \leq$ 0.92) with narrow compositional distributions as revealed by sharp superconducting transitions in magnetization measurements and close to 100% superconducting volume fraction. The crystals were extensively characterized by x-ray and compositional analysis, revealing monotonic evolution of the $c$-axis crystal lattice parameter with K substitution. Quantitative measurements of the temperature-dependent in-plane resistivity, $\rho(T)$ found doping-independent, constant within error bars, resistivity at room temperature, $\rho(300K)$, in sharp contrast with significant doping dependence in electron and isovalent substituted BaFe$_2$As$_2$ based compositions. The shape of the temperature dependent resistivity, $\rho(T)$, shows systematic doping-evolution, being close to $T^2$ in overdoped and revealing significant contribution of the $T$-linear component at optimum doping. The slope of the upper critical field, $d H_{c2}/dT$, scales linearly with $T_c$ for both $H\parallel c$, $H_{c2,c}$, and $H \parallel ab$, $H_{c2,ab}$. The anisotropy of the upper critical field, $\gamma \equiv H_{c2,ab} / H_{c2,c}$ determined near zero-field $T_c$ increases from $\sim$2 to 4-5 with increasing K doping level from optimal $x \sim$0.4 to strongly overdoped $x$=1.
• ### Temperature-concentration phase diagram of (Ca1-xLax)10(Pt3As8)(Fe2As2)5 superconductors(1212.4104)

Single crystals of (Ca1-xLax)10(Pt3As8)(Fe2As2)5 (x = 0 to 0.182) superconductors have been grown and characterized by X-ray, microprobe, transport and thermodynamic measurements. Features in the magnetic susceptibility, specific heat and two kinks in the derivative of the electrical resistivity around 100 K in the x = 0 compound support the existence of decoupled structural and magnetic phase transitions. With La doping, the structural/magnetic phase transitions are suppressed and a half-dome of superconductivity with a maximal Tc around 26 K is observed in the temperature-concentration phase diagram.
• ### Control of magnetic, non-magnetic and superconducting states in annealed Ca(Fe$_{1-x}$Co$_{x}$)$_{2}$As$_{2}$(1204.5457)

April 24, 2012 cond-mat.supr-con
We have grown single crystal samples of Co substituted CaFe2As2 using an FeAs flux and systematically studied the effects of annealing/quenching temperature on the physical properties of these samples. Whereas the as-grown samples (quenched from 960C) all enter the collapsed tetragonal phase upon cooling, annealing/quenching temperatures between 350C and 800C can be used to tune the system to low temperature antiferromagnetic/orthorhomic or superconducting states as well. The progression of the transition temperature versus annealing/quenching temperature (T-T$_{anneal}$) phase diagrams with increasing Co concentration shows that, by substituting Co, the antiferromagnetic/orthorhombic and the collapsed tetragonal phase lines are separated and bulk superconductivity is revealed. We established a 3D phase diagram with Co concentration and annealing/quenching temperature as two independent control parameters. At ambient pressure, for modest x and T$_{anneal}$ values, the Ca(Fe1-xCox)2As2 system offers ready access to the salient low temperature states associated with Fe-based superconductors: antiferromagnetic/orthorhombic, superconducting, and non-magnetic/collapsed tetragonal.
• ### Synthesis and physical properties of the new potassium iron selenide superconductor K0.80Fe1.76Se2(1201.0953)

Jan. 5, 2012 cond-mat.supr-con
In this article we review our studies of the K0.80Fe1.76Se2 superconductor, with an attempt to elucidate the crystal growth details and basic physical properties over a wide range of temperatures and applied magnetic field, including anisotropic magnetic and electrical transport properties, thermodynamic, London penetration depth, magneto-optical imaging and Mossbauer measurements. We find that: (i) Single crystals of similar stoichiometry can be grown both by furnace-cooled and decanted methods; (ii) Single crystalline K0.80Fe1.76Se2 shows moderate anisotropy in both magnetic susceptibility and electrical resistivity and a small modulation of stoichiometry of the crystal, which gives rise to broadened transitions; (iii) The upper critical field, Hc2(T) is ~ 55 T at 2 K for H||c, manifesting a temperature dependent anisotropy that peaks near 3.6 at 27 K and drops to 2.5 by 18 K; (iv) Mossbauer measurements reveal that the iron sublattice in K0.80Fe1.76Se2 clearly exhibits magnetic order, probably of the first order, from well below Tc to its Neel temperature of Tn = 532 +/- 2 K. It is very important to note that, although, at first glance there is an apparent dilemma posed by these data: high Tc superconductivity in a near insulating, large ordered moment material, analysis indicates that the sample may well consist of two phases with the minority superconducting phase (that does not exhibit magnetic order) being finely distributed, but connected with in an antiferromagnetic, poorly conducting, matrix, essentially making a superconducting aerogel.
• ### Single crystal growth and superconductivity of Ca(Fe1-xCox)2As2(1111.7034)

Nov. 30, 2011 cond-mat.supr-con
We report the single crystal growth of Ca(Fe1-xCox)2As2 (0 <= x <= 0.082) from Sn flux. The temperature-composition phase diagram is mapped out based on the magnetic susceptibility and electrical transport measurements. Phase diagram of Ca(Fe1-xCox)2As2 is qualitatively different from those of Sr and Ba, it could be due to both the charge doping and structural tuning effects associated with Co substitution.
• ### Doping - dependent superconducting gap anisotropy in the two-dimensional 10-3-8 pnictide Ca$_{10}$(Pt$_3$As$_8$)[(Fe$_{1-x}$Pt$_{x}$)$_2$As$_2$]$_5$(1111.1003)

Nov. 3, 2011 cond-mat.supr-con
The characteristic features of Ca$_{10}$(Pt$_3$As$_8$)[(Fe$_{1-x}$Pt$_x$)$_2$As$_2$]$_5$ ("10-3-8") superconductor are relatively high anisotropy and a clear separation of superconductivity and structural/magnetic transitions, which allows studying the superconducting gap without complications due to the coexisting order parameters. The London penetration depth, measured in underdoped single crystals of 10-3-8 ($x =$ 0.028, 0.041, 0.042, and 0.097), shows behavior remarkably similar to other Fe-based superconductors, exhibiting robust power-law, $\Delta \lambda(T) = A T^n$. The exponent $n$ decreases from 2.36 ($x =$ 0.097, close to optimal doping) to 1.7 ($x =$ 0.028, a heavily underdoped composition), suggesting that the superconducting gap becomes more anisotropic at the dome edge. A similar trend is found in low-anisotropy superconductors based on BaFe$_2$As$_2$ ("122"), implying that it is an intrinsic property of superconductivity in iron pnictides, unrelated to the coexistence of magnetic order and superconductivity or the anisotropy of the normal state. Overall this doping dependence is consistent with $s_{\pm}$ pairing competing with intra-band repulsion.
• ### Anisotropic resistivity in underdoped single crystals (Ba$_{1-x}$K$_x$)Fe$_2$As$_2$, $0 \leq x<0.35$(1106.0533)

June 2, 2011 cond-mat.supr-con
Temperature-dependent in-plane, $\rho_a(T)$, and inter-plane, $\rho_c(T)$, resistivities were measured for the iron-arsenide superconductor (Ba$_{1-x}$K$_x$)Fe $_2$As$_2$ over a broad doping range from parent compound to optimal doping $T_c\approx 38 K$, $0\leq x \leq 0.35$. The coupled magnetic/structural transition at $T_{SM}$ is clearly observed for samples with $T_c <$26 K ($x <0.25$), however its effect on resistivity is much weaker than in the electron-doped Ba(Fe$_{1-x}$Co$_x$)Fe $_2$As$_2$, and the transition leads only to a decrease of resistivity. In addition to the feature at $T_{SM}$, the inter-plane resistivity shows a maximum at $T^*\sim$200 K, which moves slightly to higher temperature with doping, revealing a trend opposite to the electron-doped materials. A smeared feature at about the same temperature is seen in $\rho_a(T)$. For $T<T^*$, the temperature dependence of resistivity shows systematic evolution and is close to linear at optimal doping. This feature, being most pronounced for $\rho_c(T)$, suggests the existence of a quantum critical point close to optimal doping.
• ### Anisotropic magnetism, resistivity, London penetration depth and magneto-optical imaging of superconducting K0.80Fe1.76Se2 single crystals(1102.1931)

March 2, 2011 cond-mat.supr-con
Single crystals of K0.80Fe1.76Se2.02 were suscessfully grown from a ternary solution. We show that although crystals form when cooling a near stoichiometric melt, crystals are actually growing out of a ternary solution that remains liquid to at least 850 C. We investigated their chemical composition, anisotropic magnetic susceptibility and resistivity, specific heat, thermoelectric power, London penetration depth and flux penetration via magneto-optical imaging. Whereas the samples appear to be homogeneously superconducting at low temperatures, there appears to be a broadened transtion range close to Tc ~ 30 K that may be associated with small variations in stociometry.